### Development and Validation of a Computational

### Approach to Predicting the Synthesis of Inorganic

### Materials

### by

### Daniil A. Kitchaev

### B.S., Chemical Engineering, California Institute of Technology (2012)

### B.S., Computer Science, California Institute of Technology (2012)

### Submitted to the Department of Materials Science and Engineering

### in partial fulfillment of the requirements for the degree of

### Doctor of Philosophy in Materials Science and Engineering

### at the

### MASSACHUSETTS INSTITUTE OF TECHNOLOGY

### February 2018

### c

### ○ Massachusetts Institute of Technology 2018. All rights reserved.

### Author . . . .

### Department of Materials Science and Engineering

### December 5, 2017

### Certified by. . . .

### Gerbrand Ceder

### Visiting Professor of Materials Science and Engineering

### Thesis Supervisor

### Accepted by . . . .

### Donald R. Sadoway

### Chairman, Departmental Committee on Graduate Students

### Development and Validation of a Computational Approach to

### Predicting the Synthesis of Inorganic Materials

### by

### Daniil A. Kitchaev

Submitted to the Department of Materials Science and Engineering on December 5, 2017, in partial fulfillment of the

requirements for the degree of

Doctor of Philosophy in Materials Science and Engineering

### Abstract

The concept of computational materials design envisions the identification of chemistries and structures with desirable properties through first–principles calculations, and the downselection of these candidates to those experimentally accessible using available synthesis methods. While first–principles property screening has become routine, the present lack of a robust method for the identification of synthetically accessible materials is an obstacle to true materials design. In this thesis, I develop a general approach for evaluating synthesizeability, and where possible, identifying synthesis routes towards the realization of target materials. This approach is based on a quasi– thermodynamic analysis of synthesis methods, relying on the assumption that phase selection is guided by transient thermodynamic stability under the conditions rel-evant to phase formation. By selecting the thermodynamic handles relrel-evant to a growth procedure and evaluating the evolution of thermodynamic boundary condi-tions throughout the reaction, I identify potential metastable end–products as the set of ground state phases stabilized at various stages of the synthesis. To validate this approach, I derive the quasi–thermodynamic influence of adsorption–controlled finite– size stability and bulk off–stoichiometry on phase selection in the aqueous synthesis of polymorphic FeS2 and MnO2systems, rationalizing the results of a range of

synthe-sis experiments. To enable this analysynthe-sis, I develop and benchmark the methodology
necessary for the reliable first–principles evaluation of structure–sensitive bulk and
interfacial stability in aqueous media. Finally, I describe a manganese oxide oxygen
evolution catalyst, whose high activity is controlled by metastable, tetrahedrally–
coordinated Mn3+ _{ions as an example of materials functionality enabled by structural}

metastability. The framework for the first–principles analysis of synthesis proposed and validated in this thesis lays the groundwork for the development of computa-tional synthesis prediction and holds the potential to greatly accelerate the design and realization of new functional materials.

Thesis Supervisor: Gerbrand Ceder

### Acknowledgments

I thank my parents, Natalia Dmitrieva and Andrei Kichaev, for teaching me how to be a functional, thought-filled human, and my family – Pavel Dmitriev, Renata Dmitrieva, Galina Kichaeva, Fljura Timasheva, and Igor Dmitriev – for helping them in this endeavour.

I am grateful to my graduate advisor, Gerbrand Ceder, as well as my undergrad-uate scientific advisor, Sossina Haile, for the countless hours they have dedicated to mentoring me, despite busy schedules, teleconferencing connection issues, and scien-tific frustrations.

I thank Stephen Dacek, William Richards and Aziz Abdellahi for teaching me how to be a theorist through our numerous office discussions and debates, and for guiding me through the vast array of computational tools necessary for this research.

This thesis would not have been possible without the insights, guidance, and data my collaborators and coauthors have shared with me. In particular, I thank Stephan Lany, Pieremanuele Canepa, John Perdew, Dane Morgan and Dan Nocera for their insights which were critical to much of the work in this thesis.

During my time in graduate school, I have had the pleasure of working on several projects outside of this thesis. I am grateful to Wenxuan Huang, Jinhyuk Lee, Riley Brandt, Rachel Kurchin, Julia Yang, Tina Chen, Zhengyan Lun, Raphaele Clement, Huiwen Ji and Alexander Urban for inviting me to work with them and exposing me to scientific topics I would not have encountered otherwise.

Finally, I thank Joanna Robaszewski for supporting me during my time in grad-uate school, at home and otherwise, tolerating the odd work hours and the frequent stress that were an unfortunate component of preparing this thesis.

## Contents

1 Introduction 15

1.1 Thermodynamics from first principles . . . 15

1.2 Computational materials design and the problem of synthesis . . . 22

1.3 A quasi–thermodynamic approach to synthesis . . . 24

1.4 Thesis summary . . . 26

2 First-principles methods for structure-sensitive thermodynamics 27 2.1 Features of exchange-correlation functionals . . . 28

2.2 MnO2 polymorphs as a benchmark system . . . 30

2.3 Computational methods . . . 31

2.4 Functional accuracy in the MnO2 system . . . 32

2.5 General performance across binary compounds . . . 38

2.6 Correction of oxidation potential error in SCAN . . . 45

2.7 Conclusion . . . 50

3 Phase selection during nucleation - the case of FeS2 51 3.1 Hydrothermal growth of FeS2 polymorphs . . . 51

3.2 Formalism and computational methods . . . 54

3.2.1 Thermodynamic model of an aqueous interface . . . 54

3.2.2 Computational implementation of the adsorption model . . . . 59

3.2.3 Solvation model . . . 60

3.2.4 Charged adsorption . . . 62

3.4 Phase selection during synthesis . . . 66

3.5 Generalizeability of the phase selection model . . . 67

3.6 Conclusion . . . 68

4 Phase selection through off-stoichiometry - the case of MnO2 71 4.1 The MnO2 family of compounds . . . 72

4.2 Formalism and computational methods . . . 76

4.2.1 Generation of A𝑥MnO2 intercalated structures . . . 80

4.2.2 Generation of hydrated A𝑥MnO2 configurations . . . 80

4.2.3 Generation of Ruetschi defects . . . 81

4.3 Thermodynamics of off-stoichiometric MnO2 . . . 82

4.4 Off-stoichiometry and MnO2 phase selection . . . 87

4.4.1 Alkali-stabilized phases: 𝛼, 𝜆, and 𝛿 . . . 87

4.4.2 Proton-stabilized phases: 𝛾 and R . . . 93

4.5 Selectivity of off–stoichiometric stabilization . . . 95

4.6 Off–stoichiometry and nucleation effects . . . 100

4.6.1 Computational methodology for interfacial energies . . . 102

4.6.2 Transition from 𝛽-MnOOH to Na-birnessite . . . 105

4.6.3 Stepwise crystallization of 𝛼-K𝑥MnO2 and 𝛽-MnO2 . . . 107

4.7 Conclusion . . . 110

5 Functionality from metastability - MnO2 based catalysis 113 5.1 Oxygen evolution catalysis . . . 114

5.2 Computatonal methods . . . 115

5.3 Impact of Mn(Td) on electronic structure . . . 117

5.4 Impact of Mn(Td) on catalyst performance . . . 121

5.5 Conclusion . . . 123

6 Concluding remarks 125

B Derivation of the reference entropy of ions in solution 143 C Example calculation of surface energy accounting for adsorption 145 D Relaxed adsorption geometries for FeS2 pyrite and marcasite 147

E Derivation of Mn-O aqueous chemical equilibria 151 F Thermal effects on MnO2 and MnOOH polymorphism 153

G Jahn-Teller distortions in Mn3+ _{compounds} _{155}

## List of Figures

1-1 Fraction of metastable materials in the ICSD . . . 23

2-1 Well-defined crystalline polymorphs of MnO2 . . . 30

2-2 Formation energies of MnO2 polymorphs . . . 33

2-3 Computed density of states for 𝛽-MnO2 . . . 35

2-4 PBE and SCAN accuracy in main group binaries . . . 41

2-5 PBE and SCAN accuracy in transition metal binaries . . . 44

2-6 Correction to SCAN for the energy of 3𝑑 metals . . . 48

2-7 Electrochemical potentials computed using SCAN . . . 49

3-1 Structure of FeS2 bulk and surface slab models. . . 54

3-2 Scheme for computing the free energy of an aqueous interface. . . 55

3-3 Surface energies of FeS2 pyrite and marcasite. . . 65

3-4 Thermodynamics of nanoscale FeS2. . . 66

3-5 Relationship between finite-size energetics and nucleation kinetics. . . 67

4-1 Common polymorphs of MnO2 and predicted sites for alkali intercalation. 73 4-2 Computed formation free energies of off-stoichiometric MnO2 . . . 83

4-3 Thermodynamics of proton incorporation into MnO2 polymorphs . . 86

4-4 MnO2 phase stability in aqueous media . . . 88

4-5 Stabilization of the 𝜏-MnO2 phase by the intercalation of Mg2+(H2O)𝑦 97 4-6 Finite–size phase stability in the Na-Mn-O-H space . . . 106

4-7 Finite–size phase stability in the K-Mn-O-H space . . . 108

5-1 Electronic structure of activated MnO*3+ 2 catalyst . . . 117

5-2 Band structure alignment between the activated and pristine birnessite 120

D-1 Relaxed dilute adsorption geometries on pyrite. . . 148

D-2 Relaxed dilute adsorption geometries on marcasite. . . 149

F-1 Finite temperature stability of MnO2 polymorphs . . . 153

F-2 Finite temperature stability of MnOOH polymorphs . . . 154

G-1 Jahn-Teller distortions in selected manganese oxides . . . 156

## List of Tables

2.1 Experimental benchmark data for MnO2 polymorphs . . . 32

2.2 Errors in the computed lattice parameters of MnO2 . . . 36

3.1 Bulk thermodynamics of pyrite and marcasite. . . 59

3.2 Surface and adsorption energetics of FeS2 in water. . . 64

## Chapter 1

## Introduction

In this chapter, I review the concept of first–principles computational materials de-sign and identify the problem of materials synthesis prediction as a critical obstacle to the practical and wide–spread realization of this vision. I begin by reviewing the general structure of density functional theory (DFT) as it is the dominant method for computing the thermochemical and electronic properties of inorganic materials. I then briefly discuss the now–established process of first–principles materials property computation, and motivate the development of a general scheme for evaluating ma-terials synthesizeability. I conclude by proposing a quasi–thermodynamic approach to understanding synthesizeability based on the behavior of several well–known poly-morphic systems. The implementation and validation of this scheme is the subject of chapters 2, 3, and 4 of this thesis.

### 1.1 Thermodynamics from first principles

The cornerstone of computational materials analysis from first–principles is density functional theory (DFT), which is a robust, scalable approach to evaluating the zero– temperature internal energy of many–electron systems at the level of quantum me-chanics. On the basis of these ground state energies, computed for a range of specially designed model systems and perturbations, it is possible to approximate the complete free energy of a many–body system and its thermodynamic properties. Thus, the

de-velopment of DFT, taken together with statistical mechanics, yields a practical model of first–principles materials thermodynamics, allowing for the predictive analysis of materials properties.

While the formulation of DFT is exact, its practical application involves numerous assumptions and approximations. Obtaining reliable energies from DFT calculations still relies on the careful construction of model systems and reference states which maximize the cancellation of systematic errors. The development and benchmarking of a number of these methods is the subject of chapter 2. In this section I present a brief overview of the formal structure of DFT, and review the common approxima-tions introduced in its practical application. This overview is largely based on the excellent tutorials published by K. Capelle[1] and K. Burke[2].

The foundation of quantum mechanics is the postulate that all properties of a system are encoded in its wavefunction Ψ(r), that is a solution to the Schrödinger equation [︂ −~2 2𝑚 ∇ 2 +𝑣(r) ]︂ Ψ(r) =𝐸Ψ(r)

for some potential 𝑣(r). While this equation is solvable for a single particle, it quickly becomes intractable for systems involving many interacting particles, such as any many–electron model of a solid material. One source of this intractability is that for a system of M particles, the wavefunction becomes a function of 3M coordinates, while the potential term becomes a sum of multi–particle interactions. For a Coulombic system, the Schrödinger Equation becomes

[︃(︃ _{𝑁}
∑︁
𝑖
−~2
2𝑚 ∇
2
𝑖 +𝑣(r)
)︃
+∑︁
𝑖<𝑗
𝑞2
|ri− rj|
]︃
Ψ(r1, r2, ..., rN) = 𝐸Ψ(r1, r2, ..., rN).

with charge 𝑄𝑘 ∑︁ 𝑖 𝑣(r) =∑︁ 𝑖,𝑘 𝑄𝑘𝑞 |ri− Rk|

Typically, one would approach this problem by diagonalizing the Hamiltonian, solv-ing for a wavefunction in an appropriate basis, and then calculatsolv-ing observables. While this approach can be applied to the many–body problem, for exact or even approximate algorithms, the computational cost of such direct calculation is too high for general use. Nonetheless, direct solutions of relatively small many–body systems through coupled–cluster, configuration–interaction, and quantum monte carlo meth-ods provide valuable benchmarking data for validating more approximate solutions.

A significant simplification of this problem is afforded by the Hohenberg-Kohn theorems[3], which state that all information pertaining to the ground–state of a system encoded in Ψ(r1, r2, ..., rN)can be exactly obtained from a simpler functional

of only the electron density 𝑛(r). Specifically, the Hohenberg-Kohn theorems reveal that a ground state electron density 𝑛0(r) corresponds uniquely to a ground state

wavefunction Ψ0(r1, r2, ..., rN) and at most one potential 𝑣(r). Consequently, all

ground state observables can also be calculated from the ground state electron density. Conveniently, the variational principle also holds for this electron density formulation

𝐸[𝑛0(r)]≤ 𝐸[𝑛′(r)]

where 𝐸0 is the ground state energy corresponding to a ground state density 𝑛0, and

𝐸[𝑛′_{]}_{is the energy of some other electron density. Thus, we can proceed from a trial}

electron density to a wavefunction to a potential, which we can use to create a new electron density, iterating until we achieve self-consistency and a minimum in energy:

𝑛(1)_{(r)}

→ Ψ(1)_{(r}

1, r2, ..., rN)→ 𝑣(1)(r)→ 𝑛(2)(r)→ ...

en-ergy, 𝑈[𝑛] is the electronic interaction enen-ergy, and 𝑉 [𝑛] is the potential, is typically solved using the Kohn–Sham approach[4]. We split the non–homogeneous, multiple– interacting–body problem into two simpler problems: one that is non–homogeneous, but also non–interacting, and one that is homogeneous, but interacting. Correspond-ingly, we split the total energy into non–interacting and interacting terms. The non– interacting terms are a sum of single–particle orbitals, while the interacting terms are captured by more complex exchange–correlation functionals. Mathematically, we split the kinetic energy 𝑇 [𝑛] into a sum of non-interacting “single-particle” kinetic en-ergies 𝑇𝑠[𝑛]and a remainder 𝑇𝑐[𝑛]. Given a set of single particle orbital basis functions

𝜑𝑖(r) that yield a density 𝑛,

𝑇𝑠[𝑛] = −~
2
2𝑚
𝑁
∑︁
𝑖
∫︁
𝑑3_{𝑟𝜑}*
𝑖(r)∇
2_{𝜑}
𝑖(r) =𝑇𝑠[{𝜑𝑖[𝑛]}]

Similarly, we split the interaction energy into an electrostatic Hartree term (purely electrostatic energy of a charge density 𝑛(r)):

𝑈𝐻[𝑛] =
𝑞2
2
∫︁
𝑑3𝑟
∫︁
𝑑3𝑟′𝑛(r)𝑛(r
′_{)}
|r − r′_{|}

and a remainder 𝑈𝑥𝑐[𝑛], which we group with 𝑇𝑐[𝑛] into a term called the

exchange-correlation energy 𝐸𝑥𝑐[𝑛]:

𝐸[𝑛] = 𝑇 [𝑛] + 𝑈 [𝑛] + 𝑉 [𝑛]

=𝑇𝑠[{𝜑𝑖[𝑛]}] + 𝑈𝐻[𝑛] + (𝑇 [𝑛]− 𝑇𝑠[𝑛] + 𝑈 [𝑛]− 𝑈𝐻[𝑛]) + 𝑉 [𝑛]

=𝑇𝑠[{𝜑𝑖[𝑛]}] + 𝑈𝐻[𝑛] + 𝐸𝑥𝑐[𝑛] + 𝑉 [𝑛]

The exchange correlation energy 𝐸𝑥𝑐 captures the energy associated with electron

ex-change 𝐸𝑥and electron correlation 𝐸𝑐. Exchange energy originates from the fermionic

repulsion between electrons, constraining the electronic wavefunction to be antisym-metric with respect to electron exchange. While this energy can be written explicitly in terms of orbitals (“Fock term” in the classical Hartree–Fock formulation), there is

no known way to write this term directly in terms of electron density. Correlation energy arises from the error associated with the fact that looking at electron density inherently considers only spatial averages and ignores the fact that individual elec-trons do interact with each other and are thus correlated.

Up to this point, DFT has been an exact reformulation of the Schrödinger equa-tion, and is generally no easier to solve than the direct minimization of the energy functional. The key element of DFT calculations is the observation that in practice, 𝐸𝑥𝑐[𝑛] is small compared to 𝑇𝑠[𝑛] and 𝑈𝐻[𝑛], and many relatively simple

approxi-mations can be used to compute it to acceptable accuracy. Assuming that we can approximate 𝐸𝑥𝑐[𝑛] with something not too complicated, we can solve the

remain-ing system usremain-ing the Kohn–Sham equation, which rewrites the multi-body problem discussed earlier as a system of non–interacting single–orbital problems with an ef-fective potential. Briefly summarizing the derivation, the minimization of the energy functional requires that:

𝛿𝐸[𝑛] 𝛿𝑛(r) = 𝛿 𝛿𝑛(r)(𝑇𝑠[𝑛] + 𝑉 [𝑛] + 𝑈𝐻[𝑛] + 𝐸𝑥𝑐[𝑛]) = 𝛿𝑇𝑠[𝑛] 𝛿𝑛(r) +𝑣(r) + 𝑣𝐻(r) +𝑣𝑥𝑐(r) = 0 Thus, we choose an effective potential 𝑣𝑠(r) = 𝑣(r) + 𝑣𝐻(r) +𝑣𝑥𝑐(r), such that the

energy is now only a function of a single–particle kinetic energy and a potential 𝑣𝑠.

Thus, we can solve the single-body Schrödinger Equation:

[−~

2

2𝑚 ∇

2_{+}_{𝑣}

𝑠(r)]𝜑𝑖(r) =𝐸𝑖𝜑𝑖

Given the complex nature of 𝑣𝑠(r), this equation is non–linear and must be solved

iteratively, where each iteration involves calculating the electron density correspond-ing to the current solution, and obtaincorrespond-ing a new potential until self–consistency is obtained. The resulting solutions yield the total energy of the system, as well as the electron density. The eigenvalues 𝐸𝑖 of the Kohn–Sham system are not generally

meaningful, with the exception of the eigenvalues corresponding to the highest occu-pied energy level and the lowest unoccuoccu-pied energy level, as they correspond exactly

to the ionization energy and electron affinity of the system.

Two important details in Kohn–Sham DFT calculations are (1) the choice of basis functions 𝜑𝑖 and (2) the use of pseudopotentials. Basis functions vary from plane

waves to more physical combinations of orbitals; in particular, the Vienna Ab-initio Simulation Package (VASP)[5, 6] used throughout this thesis relies on a plane-wave basis set. Pseudopotentials are precomputed modifications to the 𝑣(r) component of the 𝑣𝑠(r) Kohn–Sham potential that encapsulate the behavior of nuclear electrons,

such that the full Kohn–Sham equation is only solved for the valence electrons, which are both more relevant, and tend to have a smoother wavefunction, reducing the number of basis vectors needed for convergence. Common pseudopotentials are the Vanderbilt pseudopotentials [7], and a more general form of pseudopotentials with plane waves called the Projector Augmented Wave (PAW) method [8]. A significant advantage of the PAW method is that unlike pseudopotentials, which lose all wave-function information near the nuclei except the energy landscape, PAW calculations construct atom–like wavefunctions near the nuclei, and envelope functions beyond a certain radius, preserving nuclear wavefunction information.

The remaining difficulty in the Kohn–Sham scheme is the approximation to the exchange correlation energy 𝐸𝑥𝑐. A number of functionals exist to approximate this

energy, which can be derived from first principles, semi-empirical considerations, or fits to experimental data. Typically, each functional has a limited scope of chemical reactions for which it can yield reliable energies, and understanding this scope for each functional is critical to the practical use of DFT for materials simulations.

The simplest exchange–correlation functional is the local density approximation (LDA), which is based on the homogeneous electron gas. For this gas, the exchange energy is known analytically and can be applied to a non–homogeneous system by substituting 𝑛(r) for 𝑛, while the correlation energy has been tabulated from quantum

monte carlo calculations. Thus, the total functional becomes
𝐸𝐿𝐷𝐴
𝑥𝑐 [𝑛] =
∫︁
𝑑3_{𝑟(𝑒}
𝑥+𝑒𝑐)ℎ𝑜𝑚𝑜𝑔𝑒𝑛𝑒𝑜𝑢𝑠|𝑛→𝑛(r)

where 𝑒𝑥 and 𝑒𝑐 are the analytical and tabulated expressions for the exchange and

correlation energy of a homogeneous electron liquid, respectively [1]. Despite this very rough approximation, 𝐸𝐿𝐷𝐴

𝑥𝑐 achieves surprisingly good results due to a systemic

cancellation of error between the exchange and correlation parts of the energy – LDA underestimates the correlation energy, but overestimates the exchange energy in a systemic way.

The Generalized Gradient Approximation (GGA) improves on LDA by taking into account the gradient of the electron density:

𝐸𝐺𝐺𝐴 𝑥𝑐 [𝑛] =

∫︁

𝑑3_{𝑟𝑓 (𝑛(r),}

∇𝑛(r))

where the functional 𝑓 can be chosen by satifying various limiting behaviors, or through empirical fitting. The most common GGA variants are the PBE (Perdew, Burke, Ernzerhof)[9] and LYP (Lee, Yang, Parr)[10] functionals. Both GGA variants significantly improve upon LDA in the representation of covalent, ionic, metallic, and hydrogen–bonded system, although further corrections are necessary to account for medium and long–range van-der-Waals forces. The two main sources of error in a GGA are self–interaction and a necessary compromise between reproducing the limiting behavior of homogeneous electronic systems and that of sharp gradients, cor-responding to surfaces. Self–interaction arises from the fact that in a density repre-sentation, an electron is able to interact with itself, which destabilizes occupied states and reduces oxidation potentials and band gaps. Removal of self–interaction however is difficult and is currently achieved only with the use of empirical corrections. One such correction is the Hubbard 𝑈 model, which penalizes partially occupied states and thus counteracts the extra electronic repulsion from self–interaction. An alter-native method is the use of “hybrid functionals”, which introduce a contribution of

the exact–exchange Fock term into the Hamiltonian. Empirically, both methods can alleviate errors in oxidation potential and band gap, which are the most obvious con-sequences of self–interaction, but at the cost of significant computational expense, and larger errors in other material properties.

The issue of simultaneously reproducing the features of homogeneous densities and
electronic surfaces can be resolved in a more first–principles fashion by introducing the
kinetic energy of the system ∇2_{𝑛(r)} _{into the functional to form a meta-GGA. These}

functionals can satisfy all known constraints on an exchange–correlation functional and thus accurately reproduce the characteristics of all types of bonding [11, 12]. I will address one such functional in detail in chapter 2 of this thesis.

### 1.2 Computational materials design and the

### prob-lem of synthesis

With the development of reliable, first–principles models of materials with DFT, it has become possible to theorize a material with a particular crystal structure and composition and evaluate many of its chemical and physical properties, without re-quiring any new experimental data. Moreover, this analysis can be automated and repeated in a high–throughput fashion with minimal human interaction[13, 14, 15, 16]. This process is transformative for the design and optimization of materials for various functionalities, as time and resource–consuming laboratory testing can be limited to only those candidate materials which are likely to exhibit superior properties. Fur-thermore, systematic screening of poorly–explored chemical spaces can quickly and cheaply identify new materials which may be worth exploring experimentally, giving direction to the exploration of a generally combinatorially–large space of elemental compositions[15, 17, 18].

A significant obstacle to the full realization of this concept of computational ma-terials design is the question of synthetic accessibility. To experimentally realize a theorized material with favorable properties, it must be synthesized in the lab, which is often the most difficult and restrictive step in materials development. Early work in computational materials screening circumvented this problem by only ana-lyzing previously synthesized materials, searching for new high–performance materi-als among those tabulated in the Inorganic Crystal Structure Database (ICSD) [19] and other sources. The development of truly new materials from first principles has been restricted to materials computed to be thermodynamically stable, based on the assumption that thermodynamically stable materials are likely to be synthetically accessible by some process[17, 18, 20]. However, this approach suffers from two ma-jor drawbacks. First, it neglects the vast space of metastable materials, which make up approximately half of known materials based on those documented in the ICSD and computed within the Materials Project[14], as can be seen in Figure 1-1. Sec-ond, this approach does not give any insight into the processes that may be used to synthesize the target material. The resolution of these two challenges in a scalable, first–principles fashion is necessary for the practical implementation of computational design for the identification and development of new functional materials[18].

Metastable materials Stable materials 0 2 4 6 8 Number of materials (10 3 ) 1990 1995 2000 2005 2010

Year of addition to the ICSD

Figure 1-1: Fraction of stable and metastable materials in the Inorganic Crystal Structure Database (ICSD) [19], grouped by the year these materials were added to the database. Energies used here are taken from the Materials Project[14].

### 1.3 A quasi–thermodynamic approach to synthesis

The objective of this thesis is to identify and benchmark a computational scheme for the scalable prediction of synthesizeability and the identification of synthesis path-ways for inorganic, ionic materials. The question of which materials are synthetically accessible, and how they may be synthesized is a broad problem that in the most gen-eral sense requires a case–by–case analysis for each synthesis technique, taking into account features of each chemical system, thermodynamic driving forces and kinetic pathways. Such an analysis is intractable at an atomistic scale, and would be difficult to automate for high–throughput materials design. Instead of a direct simulation ap-proach, I describe a quasi–thermodynamic framework which can be used to eliminate materials unlikely to be synthesizeable, as well as identify the conditions under which synthesizeable materials would be likely to form. I will note that this question has been explored in parallel to myself by other authors, with similar conclusions to those I describe in this section[21, 22].

An initial insight into the origin of metastability can be obtained from known syn-thesis routes to common metastable materials. Some of the best known metastable materials are crystals formed geologically at high–pressure, such as diamond. These materials are thermodynamically stable under high–pressure and form deep in the Earth’s crust where such high–pressure conditions are available. After the crystals grow to macroscopic sizes however, they can be extracted from these high–pressure conditions while retaining their structure, persisting as macroscopic metastable mate-rials. Similar behavior can be seen in the formation of metastable nanocrystallites of TiO2, ZrO2 and other ceramics, where the combination of bulk and surface energies

stabilizes a bulk–metastable phase in a nanocrystalline size–regime, promoting its formation preferentially to that of the bulk–stable phase[23, 24, 25]. These examples suggest a more general hypothesis, which may serve as an initial approach to the computational analysis of synthesis: phase formation occurs under conditions where the phase in question is instantaneously stable within the thermodynamic boundary

conditions relevant to the synthesis environment.

An alternative approach to understanding synthesis is to analyze potential inter-mediate phases and transition states along a reaction pathway corresponding to the formation of a solid product. As the process evolves along its reaction coordinate, we can expect the system to choose locally low–energy configurations so as to avoid high kinetic barriers and highly unstable states. Thus, within some measure of configu-rational locality, the system minimizes its free energy, achieving a local equilibrium. The evolution of this local equilibrium along the reaction coordinate yields the same principle of quasi–thermodynamic stability: the formation of a product phase requires that this phase be related to an instantaneous equilibrium state at some point during the synthesis reaction.

This quasi–thermodynamic formulation of synthetic accessibility implies that at a minimum, a synthetically accessible phase must be stable under some conditions which can be expected during a synthesis reaction. Mathematically, there must ex-ist a set of thermodynamic boundary conditions, and thus a thermodynamic po-tential, for which the target phase is a ground state. For example, high–pressure metastable materials are ground states of the Gibbs free energy 𝐺(𝑇, 𝑃 ), at high pressure. Nanoscale–stabilized phases such as TiO2 anatase are ground states of a

thermodynamic potential 𝜓 which accounts for surface energy, constrained to small particle size: 𝜓(𝑃, 𝑇, 𝐴) = 𝑔𝑏𝑉 + 𝛾𝐴, where 𝑔𝑏 is the volumetric Gibbs free energy, 𝑃

is pressure, 𝑇 is temperature, 𝑉 is the particle volume, 𝛾 is surface energy, and 𝐴 is particle surface area[23, 24]. Thus, to identify synthesizable materials, it is necessary to search for the ground states of thermodynamic potentials across possible boundary conditions.

The correspondence between the evolving quasi–thermodynamic boundary con-ditions and the features of a real synthetic process relates the transient concon-ditions necessary to form a target phase to practical choices in synthesis design. While

high–pressure stabilization is a relatively straightforward thermodynamic handle to implement, it is much more difficult to, for example, constrain particle size for finite size stabilization. Instead, nano–scale stabilization may be controllable by engineer-ing nucleation and growth–rates, which are strongly dependent on supersaturation, temperature, the presence of heterogeneous nucleation centers. Some thermodynamic handles may simply be too difficult to control with the precision necessary to target a desired phase, in which case a phase predicted to be synthesizeable would not be accessible in practice. Thus, clearly identifying the relationship between synthetic processes and thermodynamic handles, is critical to the practical implementation of quasi–thermodynamic synthesis planning.

### 1.4 Thesis summary

In this thesis, I evaluate the ability of the quasi–thermodynamic framework described in section 1.3 to rationalize synthesis outcomes in several polymorphic systems, and provide an example of unique materials behavior enabled by metastability. In chapter 2, I develop and benchmark a number of computational methodologies well–suited to simultaneously capture the fine energetics of structure–selection, and the larger scale energetics of formation reactions. In chapters 3 and 4, I rationalize phase selection in the aqueous growth of FeS2 and MnO2 polymorphic systems through finite–size

sta-bilization and off-stoichiometry, explaining how the choice of synthesis medium drives the formation of an array of metastable products. Finally, in chapter 5, I present a new manganese oxide oxygen evolution catalyst as an example of unique materials functionality enabled by metastability. Throughout this thesis, I demonstrate the ability of the quasi–thermodynamic framework described here to reproduce synthesis results, identifying conditions necessary to synthesize metastable products in close agreement with experiment. These results lend significant support to the predictive power of the analysis presented here, and motivate further development of this theory, as well as its application to the realization of new materials.

## Chapter 2

## First-principles methods for

## structure-sensitive thermodynamics

A key prerequisite to the first–principles analysis of structure selection during synthe-sis is a reliable method for computing the relative energies of structures and identifying ground–state phases. In the first half of this chapter I identify the new Strongly Con-strained and Appropriately Normed (SCAN) [11] meta-GGA exchange–correlation functional for DFT as uniquely well suited for evaluating ground state selection among chemically similar structures. I demonstrate the superior performance of this func-tional with the particular example of MnO2 polymorphs, as well as with broad

statis-tics across polymorphs of ionic binary compounds. However, as synthesis involves the formation of a product from precursors which generally significantly differ in compo-sition, it is also necessary that we have a method which yields reliable results for total formation energies, including redox reactions. While SCAN improves upon previous non–empirical methods in reproducing total formation energies, alone it is insuffi-cient to predict synthesis conditions. In the second half of this chapter, I develop and benchmark a thermodynamic referencing scheme for SCAN which reduces the error in total formation energy to a level appropriate for analyzing materials synthesis.

The content of this chapter is based, often verbatim, on three manuscripts which are published or in preparation for publication:

∙ D. A. Kitchaev, H. Peng, Y. Liu, J. Sun, J. P. Perdew, G. Ceder. “The energetics of MnO2 polymorphs in density functional theory.” Phys. Rev. B, 93, 045132

(2016)

∙ Y. Zhang†_{, D. A. Kitchaev}†_{, J. Yang, T. Chen, S. T. Dacek, R. Sarmiento-Perez,}

M. A. L. Marques, H. Peng, G. Ceder, J. P. Perdew, J. Sun. “Efficient
first-principles prediction of solid stability: Towards chemical accuracy.” [submitted]
(2017) (†_{equal contribution)}

∙ D. A. Kitchaev, G. Ceder. “Eliminating oxidation potential error in semi–local density functional theory through thermodynamic referencing.” [in preparation] (2017)

### 2.1 Features of exchange-correlation functionals

First-principles thermodynamics has over the last decades matured into a reliable method for accessing the energetics of phase transitions and reactions in condensed matter systems. At the heart of this method lies Kohn-Sham density functional the-ory (DFT)[4], with its standard approximations to the exchange-correlation energy providing a reasonably accurate picture of electronic structure. One of the most ba-sic results that can be derived from a set of DFT calculations is the ground-state structure of a given compound under some set of conditions, usually set as zero tem-perature and pressure. However, despite the importance of accurate first-principles structure determination for both materials and property analysis[26, 27, 28, 29] this determination is often extremely difficult as the total energy differences between com-peting phases can be on the order of only a few meV per formula unit[30]. As a result, ground state structure selection is an attractive benchmark for verifying the adequacy of the physical model underlying a given approximation to the exchange-correlation energy.

improve-ment of a target property at the expense of errors elsewhere. To study the accuracy of common DFT methods for structure selection and other key properties in compar-ison to SCAN[11], we consider the GGAs PBE[9] and PBEsol[31], the Hubbard-U-corrected PBE+U and PBEsol+U[32, 33], and the hybrid of PBE with exact exchange HSE06[34, 35] functionals. This set of functionals provides a representative sample of common approaches to improving the accuracy of DFT. PBE is the base workhorse non-empirical functional most commonly used in the literature[36]. While PBE pro-vides reasonably accurate results for total energies across a wide range of chemistries, it suffers from significant electronic structure errors arising from self-interaction, as well as a tendency to disfavor density overlap between atoms (making lattice constants too long, especially in van der Waals bonded systems), originating from a compro-mise in the representation of the exchange energy of solids and molecules[9, 37, 38]. A common solution to the self-interaction problem is the empirically-fitted Hubbard U correction in PBE+U and PBEsol+U[33, 38]. The downsides of the +U approach are that it usually requires fitting to experimental data, and that it gives rise to er-rors in orbital hybridization, leading to further reduction of density overlap between atoms and errors in magnetism[39]. The density overlap problem in PBE can be resolved by restoring the second-order gradient coefficient for exchange, as is done in the PBEsol functional[31]. PBEsol improves the general energetic representation of solids and surfaces, but typically underestimates lattice parameters and overly stabi-lizes molecules[40] and solids with respect to atomization. Finally, hybrid functionals such as HSE06 attempt to improve upon the performance of PBE by introducing a fraction of exact exchange into the calculation[34, 35], which cancels some of the self-interaction error, at the cost of a significant increase in computational expense. In contrast, SCAN[11], and other meta-GGAs[41, 42, 43, 44, 11] attempt to correct the errors of PBE by introducing the orbital kinetic energy density into the functional, which allows for the simultaneous representation of extended systems and molecules, and enables SCAN to appropriately treat different chemical bonds (e.g., covalent, metallic, and even weak bonds), which no LDA or GGA can[45]. Since the design of SCAN is targeted to satisfy all fundamental constraints simultaneously, rather than

correcting specific drawbacks of PBE, we expect that SCAN would yield an overall improvement in the representation of all system properties relative to PBE, rather than the trade-offs in accuracy typical of other functionals.

### 2.2 MnO

2### polymorphs as a benchmark system

Figure 2-1: The polymorphs of MnO2 with well-defined crystalline phases. The

pur-ple and yellow atoms represent spin-up and spin-down Mn respectively, while the red atoms represent O. The magnetic orderings shown correspond to the lowest-energy configurations within PBE, PBEsol, and SCAN. Note that the space group corre-sponds to structural symmetry, neglecting reductions of symmetry from the magnetic ordering.

One particularly interesting system for investigating structure-transition energet-ics within DFT is the set of manganese oxides. The Mn-O system contains a diverse set of relatively well- characterized structures both across a range of stoichiometries (MnO, Mn3O4, Mn2O3, and MnO2), and within a single stoichiometry (pyrolusite 𝛽,

ramsdellite R, hollandite 𝛼, intergrowth 𝛾, spinel 𝜆, layered 𝛿 MnO2), as shown in

Figure 2-1. All the MnO2 polymorphs share a common basic atomic structure - small

Mn4+ _{ions in a spin-polarized 3𝑑}3 _{configuration and large, highly polarizable O}2- _{ions}

in a spin-unpolarized 2𝑝6 configuration, arranged in corner- and edge- sharing MnO 6

structures, many of which have been studied extensively for applications in energy storage, catalysis, pigmentation, etc[46, 47, 48, 49, 50, 51, 52, 53, 54].

The relative stability of the various oxidation states of Mn-O has been previously investigated within the Perdew-Burke-Erzenhof (PBE) and PBE+U forms of GGA-DFT, as well as with the exact-exchange-corrected hybrid PBE0 and Heyd-Scuseria-Erzenhof (HSE) functionals[55]. However, the energetics and properties of the poly-morphic phases of MnO2 remain unresolved in first-principles calculations[56, 57, 58].

Experimentally, it is established that pyrolusite 𝛽-MnO2 is the ground state of pure

MnO2[48], but to our knowledge no non-empirical DFT method has stabilized

𝛽-MnO2 as the ground state of the system. In this section, we resolve this problem with

the use of the recently reported SCAN meta-GGA[11] and show that the resolution of the ground state structure problem in the MnO2 system also leads to a much more

accurate representation of the basic physics of the material.

### 2.3 Computational methods

All calculations are done within the Vienna Ab-Initio Simulation Package (VASP)[5,
6], using a Γ-centered k-point grid with a reciprocal space discretization of 0.25 Å-1_{.}

For both PBE+U and PBEsol+U, we rely on the Dudarev effective-U formulation[33], applying a U=3.9 eV to the 3𝑑 states of each Mn atom, based on previous optimiza-tions for the formation energy, redox potential, and agreement with higher-order functionals[55, 59]. To obtain the total energy of each phase we choose the supercells given in Table 2.1, in all cases initializing the calculation based on experimentally re-ported geometries and relaxing the structures self-consistently within each functional. As all MnO2 phases are known to be well-represented energetically by

antiferromag-netic (AFM) orderings[55, 60, 58, 61, 62, 63, 64, 65], we ensure that the chosen supercells were compatible with all likely AFM orderings. To obtain the magnetic structure of each phase, we enumerate up to 12 of the most likely configurations,

cho-sen as the orderings with a net zero magnetic moment and highest symmetry. The magnetic structures used for HSE calculations and all analysis across all functionals are given in Figure 2-1 and are the ground state magnetic orderings for PBE, PBEsol, and SCAN, but not PBE+U or PBEsol+U, which we will address in a later section. Subsequent band structure and DOS calculations were set up using the scheme pro-posed by Setyawan and Curtarolo [66, 67], based on the self-consistently relaxed, symmetry-reduced primitive cells derived from the AFM orderings described above.

### 2.4 Functional accuracy in the MnO

2### system

Phase Lattice Parameters Volume ∆H_{f} E_{gap}
(a, b, c) (Å) (Å3_{/f.u.) (meV/f.u.) (eV)}

𝛽 4.39(1), 4.39(1), 2.871(4) 27.8(1) 0 0.27 R 9.29(3), 4.49(4), 2.857(8) 29.8(5) 56(32) 𝛼 9.80(2), 9.80(2), 2.85(1) 34.2(2) >0 𝛾 13.7(1), 2.86(1), 4.46(1) 29.2(3) >0 𝜆 5.67(1), 5.67(1), 5.67(1) 32.3(1) >0 𝛿 5.69(1), 5.69(1), 7(3)† >0 2.1‡

Table 2.1: Experimental parameters for the polymorphs of MnO2, given for the

su-percells used for total energy calculations. Uncertainty, given in parenthesis, is de-termined as the standard deviation between experimental results (𝛽, R, 𝛼), or as-sumed uncertainty from diffraction refinement (𝛾, 𝜆, 𝛿). The formation enthalpy is given with respect to 𝛽-MnO2. † The c lattice constant (interlayer spacing) in

𝛿-MnO2 is highly uncertain as all reported samples of this phase have some amount

of intercalated cations or water. ‡ The band gap for 𝛿-MnO2 measured by

Pin-aud et al. is for birnessite-type 𝛿-MnO2, but explicitly noting the absence of

mid-gap Mn3+ _{states[68], suggesting it should be similar to that of pure 𝛿-MnO}

2. Ref:

𝛽[48, 51, 69, 70, 71, 19, 72, 73, 74], R[48, 75, 76, 77, 51, 19], 𝛼[48, 78, 51, 19], 𝛾[49], 𝜆 [50], 𝛿[79, 80, 68]

The formation energies of the various MnO2phases with respect to the

experimen-tal ground state, 𝛽-MnO2, are given in Figure 2-2. While the experimental formation

enthalpies of most phases are not known, they must be positive in order for 𝛽 to be the ground state phase. It is clear that only PBEsol and SCAN even qualitatively reproduce this result, and only SCAN is able to quantitatively reproduce the

exper-imentally known formation enthalpy of R-MnO2. The fact that only PBEsol and

SCAN give qualitative agreement with experiment in terms of picking the correct ground state phase could be expected from the fact that SCAN and PBEsol are the only functionals that yield reasonably accurate descriptions of non-covalent electronic density overlaps, which are critically important for distinguishing between the various packings of MnO6 octahedra that form the diverse polymorphs of MnO2. However,

due to its ability to recognize not only weak electron density overlap but also strong chemical bonds[81], SCAN significantly improves on the successes of PBEsol, giving an altogether more accurate picture of the physics of the MnO2 system, leading to

the remarkable quantitative agreement between experiment and SCAN (∆H𝛽→𝑅 f =

54.2 meV/MnO2 from SCAN versus 56 ± 32 meV/MnO2 experimentally[48]).

Figure 2-2: Formation energies of MnO2polymorphs with respect to the experimental

ground state, 𝛽-MnO2. Only PBEsol and SCAN stabilize 𝛽-MnO2 as the ground

state phase, and only SCAN quantitatively agrees with the experimental transition enthalpy from 𝛽-MnO2 to R-MnO2. Note that the experimental ‘arrows’ drawn for

the 𝛼, 𝛾, 𝛿, and 𝜆 phases indicate that experimentally the formation energy of these phases is some unknown positive quantity.

In terms of electronic structure, all phases of MnO2 are semiconducting. However,

due to the self-interaction error present in both functionals[82], and the resulting re-duction of the calculated band gap. The empirical Hubbard U correction opens up a small band gap close to the experimental value (PBE+U: 0.20 eV, PBEsol+U: 0.28 eV, Exp: 0.27 eV[73, 74]), which could be expected as, by construction, the Hubbard U leads to the localization of carriers, flattening of 𝑑-bands, and opening of band gaps[33]. HSE in turn converges to a much larger band gap (1.7 eV), while SCAN gives a gap (0.43 eV) that is close to the +U and experimental results. The results are similar for the 𝛿 phase where the experimental band gap is also known: PBE and PBEsol underestimate the bandgap (1.1 eV and 0.96 eV respectively, versus 2.1 eV experimental [68]) PBE+U, PBEsol+U, and SCAN give almost identical band gaps in good agreement with experiment (2.0 eV, 2.1 eV, and 2.0 eV respectively), and HSE overestimates the band gap (3.4 eV). It must be noted that the experimental band gaps in the MnO2 system are not definitively established - the gaps reported here are

based on the best estimates available in the literature. The fact remains however that SCAN significantly increases the band gap compared to PBE and PBEsol, which are known to underestimate band gaps, and agrees with values obtained from empirically-fitted PBE+U and PBEsol+U functionals, while keeping the gaps well below those of HSE. The improvement in band gap could originate from two sources. First, the SCAN meta-GGA, like the hybrid functionals, is implemented in a generalized Kohn-Sham scheme in which the exchange-correlation potential is not a multiplica-tive operator[11]. Second, the self-interaction error in SCAN is greatly reduced in the case of well–localized electrons as SCAN uses a functional form that is almost self-interaction free in the case of atomic-like densities, where the exchange-correlation hole remains near its reference electron[11]. As the valence band in 𝛽-MnO2 consists

of weakly-hybridized Mn 𝑡2𝑔 and O 𝑝𝑧 states, this condition may be approximately

satisfied, leading to a cancellation of self-interaction in SCAN, and consequently an increased band-gap compared to PBE or PBEsol. We must note however that this result is somewhat atypical - we find that for many materials, including rutile TiO2,

Figure 2-3: The total and atom-projected density of states of 𝛽-MnO2. The shaded

regions denote the band gap predicted by each functional, while the dotted line marks the experimental bandgap, 0.27 eV[73, 74]. The DFT bandgap is given by the gen-eralized Kohn-Sham eigenvalues from a band structure calculation, while the DOS is calculated with a 0.1 eV smearing.

Another important property of the MnO2 system is its magnetic configuration.

Experimentally, 𝛽-MnO2 adopts a helical magnetic configuration[83, 84, 85] while all

other phases are believed to be antiferromagnetic (AFM)[62, 63, 64, 65]. In previous DFT work, the ferromagnetic (FM) form of 𝛽 and 𝛼 MnO2 was found to be stable

in PBE+U, in conflict with experiment [55, 61, 60]. We find that both PBE+U and PBEsol+U stabilize FM orderings with respect to the reference AFM configurations given in Figure 2-1, and overall favor alternate AFM configurations with clusters of nearest-neighbor aligned spins, contrary to what could be expected on the basis of oxygen-mediated superexchange governing the antiferromagnetism in MnO2. In

con-trast to the +U functionals, PBE, PBEsol, and SCAN favor the AFM configuration in 𝛽, R, 𝛼 and 𝛾, and give essentially degenerate results for the AFM and FM config-urations in 𝛿 and 𝜆, likely due to the fact that the size of the true antiferromagnetic ground state unit cell in these phases includes up to 128 spins[63, 86] the enumeration

PBE+U PBE PBEsol+U PBEsol HSE SCAN MRE 1.64% 0.64% 0.25% -0.73% -0.37% -0.51% MARE 1.64% 0.66% 0.53% 0.79% 0.62% 0.68%

Table 2.2: The lattice parameter mean (absolute) relative error (MRE, MARE) of the 𝛽, R, 𝛼, 𝛾, and 𝜆 phases of MnO2, as compared to the experimental values

presented in Table 2.1. It is clear than SCAN performs better than the similarly efficient non-empirical PBE and PBEsol functionals, and is outperformed by only HSE and the empirically fitted PBEsol+U. Note that the 𝛿 phase is excluded due to highly uncertain experimental lattice constants, as discussed in the caption of Table 2.1.

of which is beyond the scope of this work.

A final measure of functional accuracy is its ability to reproduce lattice param-eters, as they are often indicative of how well the functional captures the bonding character of the solid[87, 88]. The improved performance of SCAN with respect to lattice constants in comparison to PBE and PBEsol, as can be seen in Table 2.2, fol-lows from the fact that SCAN yields a superior description of both the bonds within the MnO6 octahedral environment and the weak electron density overlap between

oc-tahedra. It is worth noting the exceptional performance of PBEsol+U in reproducing the lattice constants here. While PBEsol underestimates lattice constants, the +U modification typically leads to larger lattice parameters by reducing the electronic overlap between atoms, counteracting the error in PBEsol. Consequently, PBEsol+U is able to minimize the lattice constant error for an optimal choice of U-value[58].

For all the properties of MnO2 that we have considered (polymorph formation

energy, band gap, magnetization, and lattice constants), SCAN is the only functional to give high-quality, ab-initio results in agreement with experiment across the board. In contrast, the empirically-fitted PBEsol+U functional performs as well as or bet-ter than SCAN on band gaps and lattice constants, but mispredicts the polymorph order and the magnetic character of the system. PBEsol performs well on the poly-morph order and magnetization, but significantly underestimates lattice constants and band gaps. HSE, while being much more computationally expensive than all

other functionals tested here, only performs well on lattice constants. The consis-tent agreement between SCAN and experimental results across multiple properties suggests that SCAN, more so than other functionals, is able to capture the physics governing the system rather than acting as a fortuitous correction that improves a target property. We propose that the reason for this superior and consistent per-formance lies in the design features of SCAN - its built-in agreement with numerous limiting constraints on the exchange-correlation energy, and the inclusion of appropri-ate norms for which semi-local functionals can be exact or nearly-exact, which serve to guide the functional from one constraint to another. We expect similarly positive results on other transition metal oxides with high-spin configurations and less-than half-full 𝑑 shells, and somewhat worse results in more self-interaction-dominated sys-tems. However, much more extensive calculations are needed to fully explore the accuracy of SCAN across other chemical spaces.

In conclusion, we have investigated the accuracy of several common DFT func-tionals, as well as the recently introduced SCAN meta-GGA, with respect to their ability to reproduce key properties of the challenging MnO2 system. Specifically, we

looked at the relative stability, band gaps, magnetic structure, and lattice constants of the 𝛽, R, 𝛼, 𝛾, 𝜆, and 𝛿 phases on MnO2. We found that although each

indi-vidual property can be reproduced to good agreement with experiment by several functionals, only SCAN gives quantitatively reliable results for all properties at once. The accuracy, reliability, and computational efficiency of this new functional opens the door to the rigorous theoretical study of the manganese oxide system, from its still-uncertain basic physics to the complex mechanisms underlying the rich catalytic, electrochemical, and optoelectronic behavior of this material.

### 2.5 General performance across binary compounds

Generalizing from the favorable performance of SCAN in reproducing the properties and energetics of MnO2 polymorphs, we examine the performance of this exchange–

correlation functional more broadly, focusing specifically on the question of phase stability across binary ionic compounds. The ability to evaluate chemical stability, i.e., whether a stoichiometry will persist in some chemical environment, and struc-ture selection, i.e. what crystal strucstruc-ture a stoichiometry will adopt, is critical to the prediction of materials synthesis[89], reactivity[26, 27] and properties[53]. We demonstrate that SCAN[11] is able to address both facets of the stability problem reliably and efficiently for main group compounds, while transition metal compounds are improved but remain a challenge. SCAN therefore offers a robust model for a significant portion of the periodic table, presenting an opportunity for the develop-ment of novel materials and the study of fine phase transformations even in largely unexplored systems with little to no experimental data.

For known materials, the question of solid phase stability can be resolved exper-imentally through a variety of calorimetric techniques, which yield the enthalpy of formation(∆H𝑓). In the prediction of new materials however, the formation enthalpy

must be calculated from first-principles, which is most commonly done using DFT with the well-established Perdew-Burke-Ernzerhof (PBE)[9] density functional. Fur-thermore, in the evaluation of solids differing in structure, but not chemistry, the differences between the formation enthalpies of competing phases often lie on a very fine energy scale, and are very difficult to measure experimentally, motivating their calculation from first-principles[90].

Due to the diversity of chemical degrees of freedom, from subtle structural differ-ences to changes in bonding characteristics, it is challenging for first-principles meth-ods to tackle both facets of the stability problem at reasonable computational cost. High–level wavefunction methods[91] (e.g., the configuration interaction or quantum

monte carlo approaches) can achieve accuracy comparable to calorimetry, but they are limited to systems having a relatively small number of electrons per periodic unit cell due to their high computational cost. DFT[4, 92, 93, 94], with the PBE[9] gen-eralized gradient approximation to its exchange-correlation energy currently is the dominant approach for calculation due to its relatively cheap computational cost and reasonable accuracy. Unfortunately, errors in formation enthalpy predicted by PBE are usually at the level of ≈0.2 eV/atom (see Figure 2-4), which is not sufficient for the comparison of competing formation reactions, especially those leading to chemically similar solids. We find that SCAN[11] halves the errors of PBE in predicting forma-tion enthalpies of about 200 binary solids[95], while retaining a comparable efficiency to PBE. Remarkably, SCAN also yields a significant improvement in the reliability of crystal structure selection, consistently halving the error rate in ground state selection accuracy and reducing the error in the relative energies of crystal structures. While the computational cost of SCAN is modestly greater than (usually 2 to 3 times) that of PBE, it is much less (in general by an order of magnitude in plane-wave codes) than that of hybrid functionals, and very much less than that of wavefunction methods.

To systematically compare the behavior of SCAN and PBE, we group chemistries by how they are affected by known errors in semi-local density functionals. The three major sources of error in PBE are the self-interaction error (SIE), the incomplete error cancellation between the target compound and the elemental references, and the absence of van der Waals interactions. SIE is intrinsic to all semi-local density functionals, among which are PBE and SCAN. SIE manifests itself in transition metal compounds, especially in semiconducting and insulating oxides, more than in main group compounds due to the presence of valence 𝑑 electrons that localize more than valence 𝑠𝑝 electrons[37]. The late 3𝑑 elements Cr, Mn, Fe, Co, and Ni are especially problematic. To resolve SIE in true first-principles spirit, non–local corrections are necessary, which are typically computationally expensive and scale poorly with sys-tem size. Therefore, we first address the behavior of main group compounds so as to characterize the performance of PBE and SCAN as efficient semi-local functionals

largely in the absence of SIE.

The evaluation of the enthalpy of formation is based on 196 binary compounds
with 101 main group systems and 95 systems containing transition metals (see
Ap-pendix A). The analysis of structure selection accuracy is based on 297 ionic binary
chemistries, of which 191 are main group compositions and 106 contain transition
metals (see Appendix A). In the choice of chemistries, we choose only compositions
for which the low-temperature, low-pressure ground-state crystal structure is known
experimentally. The chemistries included in this sample are comprised of
compo-sitions chosen to benchmark formation enthalpy, AB-type ionic compounds, and a
selection of binary compositions previously enumerated in crystal structure
predic-tion studies[20]. To the best of our knowledge, this selecpredic-tion of chemistries does not
introduce any bias in the likelihood of structure selection error not present more
gen-erally in binary main group and transition metal compounds. For each chemistry,
we consider experimentally reported crystal structures from the Inorganic Crystal
Structure Database[19], as well as likely structures predicted by data mined
elemen-tal substitution methods[20], giving a toelemen-tal of 3026 cryselemen-tal structures. Finally, to
determine whether or not a DFT-relaxed crystal structure matches the
experimen-tally reported structure, we rely on a distortion-tolerant affine map, implemented as
the StructureMatcher algorithm in the Pymatgen package[96]. All calculations are
performed using the Vienna Ab-Initio Simulation Package (VASP)[5, 6] using the
projector augmented wave (PAW) method[8] with a reciprocal space discretization
of 25 Å1 _{and a plane wave energy cutoff of 520 eV. In magnetically active systems,}

the energy is taken as the lowest of a ferromagnetic and a sample of small–unit–cell
antiferromagnetic orderings. All calculations are converged to 106 _{eV in total energy}

and 0.01 eV/Å on atomic forces.

As shown in Figure 2-4a, the mean absolute error (MAE) of SCAN in the forma-tion enthalpy of 102 main group compounds is 0.084 eV/atom, about 2.5 times lower than that of PBE, while the MAE of SCAN for the 21 main group oxides shown in

Expt

PBE

SCAN MAE (eV/atom)

PBE
SCAN
Oxides Overall
0.293 0.217
0.038 0.084
-4 -3 -2 -1 0
∆HExpt _{(eV/atom)}
∆H
DFT
(eV/atom)
-4
-3
-2
-1
0
Oxides
-3 -2 -1
-3
-2
-1
Main group
compounds
a. b.

Tolerance in ground state energy (eV/atom) 0.0% -0.05 -0.04 -0.03 -0.02 -0.01 0 5.0% 10.0% 15.0% 20.0% 25.0% Fr equen cy of gr oun d stat e mis pr ed ic tio n PBE SCAN Main group compounds

Figure 2-4: SCAN provides a significant improvement over PBE in computing the absolute and relative stability of main group compounds. a. The formation enthalpy of main group compounds, and oxides in particular. b. The probability that the computed energy of a predicted structure with respect to that of the experimental ground state structure lies below a threshold energy or tolerance across main group compounds, for a range of tolerances.

the inset is 0.038 eV/atom. The reduction in error afforded by SCAN relative to PBE originates from the fact that PBE is not able to simultaneously and accurately treat the different types of chemical bonds[11, 12] (covalent, metallic, ionic, hydrogen, and van der Waals) found in a compound and its constituent elemental phases, leading to the well-known imperfect error cancellation, e.g., between the molecular O2

refer-ence and metal oxides[59]. SCAN, on the other hand, is able to capture the behavior of all such interactions by introducing the Kohn-Sham kinetic energy density into the functional in a way that satisfies all known limiting behaviors and constraints on electronic interaction appropriate to semilocal functionals[11]. This construction leads to a widely-predictive functional[97]. In particular, without being fitted to any bonded system, SCAN captures even the intermediate-range van der Waals attrac-tion between neighboring atoms in a solid, which PBE largely neglects. Furthermore, PBE underestimates the chemical stabilities of most solids, for example erroneously making InN chemically unstable, an error which SCAN avoids. These errors arise largely from PBE’s over-stabilization of reference molecules, and could not be fixed by simply adding a van der Waals correction to PBE.

An even stronger indication of the general reliability of SCAN for stability
cal-culations is its superior performance in identifying ground state crystal structures.
Here the intermediate-range van der Waals interaction, present in SCAN but not in
PBE, can play a particularly important role, for example by stabilizing the correct
CsCl structure in the heavy halides CsCl, CsBr, and CsI. Based on 191
stoichiomet-ric main group binary compounds with 1659 experimentally-reported and predicted
crystal structures, we identify the most stable low-temperature, low-pressure phases
within PBE and SCAN. We then evaluate the frequency with which PBE or SCAN
stabilizes an incorrect ground-state structural polymorph in comparison to the
ex-perimental structure. The zero-temperature ground state crystal structure is
ther-modynamically defined as the phase of lowest enthalpy, as, under these conditions,
enthalpy is exactly equal to the system Gibbs free energy. Thus, the relative
zero-temperature DFT-computed energies of competing crystal structures provide a nearly
complete representation of their relative Gibbs free energies under these conditions,
omitting the change in zero-point vibrational energy which is on the scale of 0.005
eV/atom[98, 99, 100, 101], ambient pressure effects, which lie on the scale of 0.001
eV/atom, and smaller contributions. To account for these effects, as well as other
potential noise in the calculations, we introduce a tolerance on structure selection
∆E_{tol}, and count the frequency with which PBE or SCAN erroneously stabilize a
crystal structure by more than ∆Etol with respect to the experimental ground state

structure. As can be seen in Figure 2-4b, SCAN provides a significant improvement over PBE in selecting the correct ground state structure, reducing the frequency of structure prediction error from 12% to just 3% at a 0.01 eV/atom tolerance, where the improvement in structure selection accuracy likely originates from the more accurate physical model provided by SCAN relative to PBE. Notably, as the energy scale of competing crystal structures[24, 22, 30] is far below the average error suggested by total formation enthalpy statistics discussed earlier, it is evident that reliable struc-ture selection is a sensitive indicator of how well a functional capstruc-tures fine details in the relative stability of chemically-similar phases.

These structure selection results highlight the difficulty of reliable structure pre-diction in first-principles calculations. While PBE yields close to a 21% error rate in structure selection in absolute terms and a 12% error rate with a 0.01 eV/atom tolerance, this error rate is likely a lower bound as no method we are aware of can guarantee that no other crystal structures exist with a lower energy for any given chemistry. Conversely, experimental uncertainties in ground-state crystal structure originating from difficult to observe low temperature phase transitions, small off sto-ichiometries, and other errors mean that even the exact functional would likely not be able to achieve complete agreement with experiment. In this light, SCAN’s 3% error rate within the 0.01 eV/atom tolerance is remarkable. The impact of this im-provement is immediately visible - for example, in SiO2, SCAN is necessary to

repro-duce the correct 𝛼-quartz low-temperature, low-pressure ground state structure, and correspondingly, the pressure-temperature phase diagram, as PBE overstabilizes the high-temperature 𝛽-cristobalite polymorph. The intermediate-range van der Waals interaction in SCAN stabilizes the correct, higher-density quartz phase of this earth-abundant material. Taken together with the promising performance in predicting formation enthalpy, these results suggest that SCAN is highly reliable for both the absolute and relative stability of the main group compounds.

We now turn to transition metal compounds, where self-interaction error poses a fundamental limitation on the performance of semi-local density functionals. For the formation enthalpies of 98 transition metal binaries, Figure 2-5b shows that SCAN still has an MAE of 0.122 eV/atom, which is significantly larger than that of the main group compounds. However, SCAN still improves over PBE by about 0.08 eV/atom, or 40% of the total PBE error, for the transition metal compounds. Similarly, as can be seen in Figure 2-52b, based on 106 transition metal binary compounds with 1366 experimental and predicted structures, SCAN still gives a significant improvement relative to PBE in structure selection accuracy, although the absolute performance of both functionals is much worse than that in the main group compounds, both in the

a.
Expt
PBE
SCAN
Oxides
MAE (eV/atom)
PBE
SCAN
Oxides Overall
0.289 0.204
0.175 0.122
Transition metal
compounds
-4 -3 -2 -1 0
∆HExpt _{(eV/atom)}
∆H
DFT
(eV/atom)
-4
-3
-2
-1
0
-3 -2 -1
-3
-2
-1
-4
-4
b.

Tolerance in ground state energy (eV/atom) 0.0% -0.05 -0.04 -0.03 -0.02 -0.01 0 10.0% 20.0% 30.0% Fr equen cy of gr oun d stat e mis pr ed ic tio n PBE SCAN Transition metal compounds

Figure 2-5: SCAN considerably reduces the average error in formation enthalpy and structure selection error frequency relative to PBE in transition metal compounds, which are more difficult than are the main group compounds due to the increased contribution of the self-interaction error. (a.) The enthalpy of formation of transition metal binary compounds, and oxides in particular. (b.) The probability of incorrect structure selections by PBE or SCAN across transition metal compounds, for a range of tolerances.

frequency of structure selection errors and their energetic magnitude. The fact that this discrepancy persists even at a 0.02 eV/atom tolerance, where the SCAN error rate in main group chemistries approaches zero, suggests that further improvements in functional performance would require a fundamentally different approach, moving to non-local functional forms or explicit self-interaction corrections[102, 103, 104].

A number of different approaches have been developed to deal with the imper-fect error cancellation of PBE, such as the fitted elemental-phase reference energies (FERE) scheme[105], and other schemes with fitted corrections to elemental and molecular reference states[59, 106]. These corrections assume that most of the error in compound formation enthalpy depends only on the overall composition, and at-tempt to eliminate this error by using the total energies of elemental phases as fitting parameters. In the case of FERE, with about 30 fitting parameters, the PBE MAE is reduced from 0.250 eV/atom to 0.052 eV/atom for a set of 110 main-group binary solids which largely overlaps our testing set. However, neither FERE nor the other composition-based schemes can provide the correction to PBE needed to predict the